International Journal of Scientific Engineering and Technology www.ijset.com, Volume No.1, Issue No.2 pg:112117
(ISSN : 22771581) 01 April 2012
Life Prediction and crack propagation analysis for the Pipe weld Straight component (PWSC) of power plant Shrikrishna Dhakad1, Dr.Sanjeev Saxena2 Dr.Geeta Agnihotri3 1
2
SAT I (deg. ), college, Vidisha (M.P.), 464001,sk27_dhakad@yahoo.com Advanced Materials and Processes Research Institute (AMPRI), Bhopal 462 026. san_bpl@yahoo.com 3 MANIT, Bhopal , professor in the mechanical Engg. Deptt. agnihitrig@manit.ac.in
Abstract: In the present paper the fatigue crack growth behavior of surface cracked piping component are performed on the basis of the linear elastic fracture mechanics (LEFM) principles with particular interest in its ability and accuracy to predict full scale component tested experimental data. The crack prorogation is consider in semi elliptical shape. In the present paper three different diameter Pipe weld straight components (PWSC 126, PWSC 164, PWSC 165) are selected. The two SIF solution (ASM and Bergman) available in the literature, the extreme point SIFs (depth and surface) are determined at initial crack depth of 3.6 mm the case PWSC126. The yield strength for the material is 325MPa. In this case, the applied nominal 183MPa stress range, which is 0.56 times the strength of the material. Therefore, for the particular case the plastic zone correction is applied. The two extreme points SIFs are determined at physical crack depth and also at effective crack length. The details of crack depths at which these SIFs are determined are given in Table 1 and Table 2 Corresponding crack lengths determined are also given in these tables. The analysis are also done for remain two pipe , having the different yield strength of the materials. The details of crack depths at which these SIFs are determined are given in Table 3&4 and Table 5&6 Corresponding crack lengths determined are also given in these tables. Keywords: Fatigue; Paris equation; Stress intensity factor solution; Crack growth behavior; Power plant component
Introduction: The present work has been carried out to assess the prediction accuracy of crack growth behavior of experimentally tested fullscale pipe component having outer surface crack in circumferential direction. In case of the studied pipes, two stress intensity factor (SIF) solutions are available in the literature. One is given in
112
ASM Handbook Vol. 19 [1] appendices based on Mettu SR et al. numerical work and other one proposed by Bergman [2] based on 3D FEM solution using ABAQUS code. These SIF solutions are for semielliptical crack profile. In the experimental pipe specimens the initial crack geometry is having a constant depth.. As the SIF solutions for constant depth crack profile are not available in the open literature. In the present work the SIF solutions available in the literature (ASM handbook [1] and Bergman solution [2]) are evaluated to predict the component behaviour using the fracture specimen tested data. Though, the crack profile in the two available SIFs solutions [1, 2] are different than that of experimental study specimen’s crack profile, these have been used to understand the effect of assumed crack profile in the predicted results. The present study have been done on material used in Indian nuclear power plant component.
2. Experimental tested data 2.1 Material properties The tensile properties of SA333Gr.6 carbon steel base material tested at room temperature have been considered in the present study. The material Young’s modulus is 203Gpa and the Yield strength is 302MPa, ultimate tensile strength is 450MPa & Poisson’s ratio 0.3. The fatigue crack growth tests were reported [3] to be conducted on the standard three point bend fracture specimen. The material constants of Paris crack growth law had been evaluated by fitting the test data points that is giving in the form of equation below as shown in Table 2.1. Table 2.2 showed the material fatigue data for base and weld metal for the material studied. Table 2.1 Tensile properties of SA333Gr.6 carbon steel tested at room temperature
International Journal of Scientific Engineering and Technology www.ijset.com, Volume No.1, Issue No.2 pg:112117 Mate rial
Yield strengt h Y (MPa)
Ultimate tensile strength (MPa)
Elon gatio n (%)
% reduc tion in area
E(G Pa)
µ
302
450
36.7
72.96
203
0.3
Weld
325
466
18.7

203
0.3
Table 2.2 Paris constant values for the material studied
406mm pipe 219mm pipe 406mm pipe 219mm pipe
Notch locatio n
Paris constant C (mm)
M
0.1
Base
8.87 x 1010
3.80
0.1
Base
3.807 x 109
3.034
0.5
Weld
6.98 x 1010
3.650
0.5
Weld
4.279 x 109
2.9039 7
In the present study, three different outer diameter pipes having 219 mm, 324mm and 406 mm used in the piping system of Indian PHWRs have been used for test. The pipe specimens have surface notches of different sizes machined at the outer surface in the circumferential direction by a milling machining process. The experimental data gathered from the literature for the present study are shown in Table 2.3
da 3.03445 3.807 x109 K dN (1)
Here da / dN is in m/cycle and K is in MPa m . The fullscale pipe used in the primary heat transporting system of Indian nuclear power plant has been taken in the present study [4].
Methodology used: With the use of crack growth laws it is possible to predict the life of the piping component subjected to fatigue. For a structure under fluctuating loads, the crack growth rate can be related to the variation of SIF, K, during a load cycle. K has considerable influence on fatigue crack growth and if K remains constant, the crack growth rate is also constant. Paris has expressed the relationship between crack growth
113
da
C K d
m
(3)
Kd – SIF range at deepest point of surface crack m (4) dc dN CK c where dc  Extension of crack length and Kc  SIF range at surface crack tip. The computation of crack propagation along the two directions has to be carried out simultaneously since Eqns.(3) &(4) are not independent. Now the new dimensions of the crack are calculated as: (5) anew aold da
2cnew 2cold dc
2.3 Pipe specimen test data
(2)
Where C and m are crack growth constants and K= KmaxKmin. The quantities Kmax and Kmin are the SIF values corresponding to the maximum and minimum stress levels in the fatigue load cycles. For the assumed initial crack depth, the number of cycles required for the incremental increase in crack depth can be calculated as follows from Eqn.(3)
dN
Stres s ratio
for stress ratio (R) = 0.1
rate (da/dN) and K as a power law in the following form:
da m C K dN
Base
Pipe case
(ISSN : 22771581) 01 April 2012
(6)
The process is repeated until the crack reaches throughthickness or K reaches fracture toughness of the material. For every incremental increase in crack depth, the life cycles are calculated using Eqn.(3) and added upto throughthickness, to give the total life of the piping component corresponding to throughthickness crack.( LEFM).SIF is measure if the stress surrounding the crack tip of a body and is K=fx bx( a)0.5 ( 7) Where f is the function that depend on the geometry of the crack and cracked part under consideration. A is the crack size and b is the nominal stress action normal to the crack.The geometry factor f find from ASM E  647 and data book with the help of experimental tested solution available different problem. By calculating the SIF, the process of crack growth can be determined. If the SIF is lower than the threshold value no crack propagation is expected. The SIF excesses the upper material value Kc called fracture toughness the crack propagation is unstable with cause failure of the components. In the range between these two limits stable crack grow can be observed. If the value of bending stress ( b) is more then 30 to 40 % yield strength of material ( y). aeff.=a+1/3 (kd/ y)2 (8)
International Journal of Scientific Engineering and Technology www.ijset.com, Volume No.1, Issue No.2 pg:112117 2ceff=2c+2/3 ( ks/
y)
2
(9)
da – Assumed increase in crack depth.
50 Stress intesity factor (MPa Vm)
Then the extension of crack length at the surface can be calculated by putting the number of cycles obtained from Eqn.(4) to the following equation: Using two SIF solutions the extreme point SIFs are calculated at initial crack geometry(initial crack length) in mm , crack depths and new lengths are calculated for each increase in crack depth. The process is repeated until the crack reaches throughthickness. prediction results using ASM & MBargman solution for(PWSC 126, PWSC 164, & PWSC 165) are shown in Tables 4.1& 4.2 for the PWSC 126.
45
Fig.1 showed the variation of SIF solution with crack depth predicted by two SIF solution considered in the present study. The depth position SIF values SIF values predicted by Bergman solution compares well with that by ASM solution. Similarly, the surface position SIF predicted by Bergman SIF solution compares well initially with ASM handbook SIF solution thereafter Bergman solution gives higher predicted value of SIF as compared to ASM predicted value.Fig.2 showed the comparison of predicted crack growth behaviour with experimental results, Fig. 3 Variation of crack length with fatigue cycles, Fig. 4 Variation of aspect ratio with fatigue cycles& Fig. 5Variation of aspect ratio with crack depth
ASM Kdeff
35
ASM Ks
30
ASM Kseff
25
Berg Kd
20
Berg Kdeff
15
Berg Ks
10
Berg Kseff
5 0 0
0.2
0.4 0.6 0.8 Crack depth/ thickness (a/t)
1
1.2
Fig. 1 Variation of SIF range with crack depth for pipe case PWSC126
Crack depth/ thickness (a/t)
1 0.8 0.6 0.4 Prediction ASM Prediction Berg
0.2
Experimental
0 0
25000
50000
75000
100000
Number of cycles
Fig. 2 Variation of a/t with fatigue cycles for pipe case PWSC126 80
Prediction ASM 75
Crack length (2c) in mm
Using the methodology described in chapter 3 and two SIF solution (ASM and Bergman) available in the literature, the extreme point SIFs (depth and surface) are determined at initial crack depth of 3.6mm the case PWSC126. The yield strength for the material is 325MPa. In this case, the applied nominal 183MPa stress range, which is 0.56 times the strength of the material. Therefore, for the particular case the plastic zone correction is applied. The two extreme points SIFs are determined at physical crack depth and also at effective crack length. The details of crack depths at which these SIFs are determined are given in Table 4.1 and Table 4.2 Corresponding crack lengths determined are also given in these tables. The determined SIF range for the case is found lesser than the fracture toughness of the material. Therefore, using Paris equation, the crack growth prediction process is repeated upto throughwall crack depth.
ASM Kd
40
4.Result and discussion
114
(ISSN : 22771581) 01 April 2012
Prediction Berg Experimental
70 65 60 55 50 0
20000
40000
60000
80000
100000
Number of cycles
Fig. 3 Variation of crack length with fatigue cycles for pipe case PWSC126
International Journal of Scientific Engineering and Technology www.ijset.com, Volume No.1, Issue No.2 pg:112117
(ISSN : 22771581) 01 April 2012
15 144
10
Prediction Berg
142
Experimental
140
Prediction ASM Prediction Berg
Crack length(2c)
Aspect ratio (2c/a)
Prediction ASM
5
Experimental
138 136 134 132
0
130
0
20000
40000
60000
80000
100000
0
5000
10000
Number of cycles
15000
20000
25000
30000
35000
Number of cycles
Fig. 4 Variation of aspect ratio with fatigue cycles for pipe case PWSC126
Fig. 8Variation of crack length with fatigue cycles
Prediction ASM
25
Prediction Berg
10
Prediction ASM 20
Experimental
5
0 0
0.2
0.4
0.6
0.8
1
15
10
5
Crack depth/thickness (a/t)
0 0
Fig. 5Variation of aspect ratio with crack depth for pipe case PWSC126
5000
15000
20000
25000
30000
35000
Number of cycles
80
25
70
Prediction ASM
50 40 30 20
Aspect ratio(2c/a)
ASMKd ASMKdeff ASMKs ASMKseff Berg Kd Berg Kdeff Berg Ks Berg Kseff
60
10
Prediction Berg
20
Experimental 15 10 5 0
0 0
0.5
1
1.5
0
0.2
Crack depth/thickness (a/t)
0.4
0.6
0.8
1
Crack depth/thickness (a/t)
Fig. 6 Variation of SIF range with crack depth
Fig.10 Variation of aspect ratio with crack depth
case PWSC 165
1 0.9
60
0.8
Stress intensity factor (MPa Vm)
Crack depth/thickness (a/t)
10000
Fig. 9Variation of aspect ratio with fatigue cycles
case PWSC 164 Stress intensity factor (MPa Vm)
Prediction Berg
Experimental
Aspect ratio(2c/a)
Aspect ratio(2c/a)
15
0.7 0.6 0.5 0.4 0.3 Prediction ASM
0.2
Prediction Berg
0.1
Experimental
ASMKd ASMKdeff ASMKs ASMKseff Berg Kd Berg Kdeff Berg Ks Berg Kseff
50
40
30
20
10
0 0
5000
10000
15000
20000
25000
30000
35000
Number of cycles
Fig. 7 Variation of crack depth/ thickness with fatigue cycles
115
0 0
0.2
0.4
0.6
0.8
1
1.2
1.4
Crack depth/thickness (a/t)
Fig. 11Variation of SIF range with crack depth
International Journal of Scientific Engineering and Technology www.ijset.com, Volume No.1, Issue No.2 pg:112117
(ISSN : 22771581) 01 April 2012
1
Crack depth/thickness (a/t)
0.9
Pipe case
0.8 0.7 0.6 0.5
Prediction ASM Prediction Berg Experimental
0.4 0.3 0.2 0.1 0 0
10000
20000
30000
40000
50000
60000
Number of cycles
Fig. 12 Variation of crack depth/ thickness with fatigue cycles 80
Prediction ASM Prediction Berg Experimental
Crack length (2c) in mm
78 76 74 72 70 68 66 64 0
10000
20000
30000
40000
50000
60000
Number of cycles
Exp.
PWSC 126 77.4 PWSC 140.4 164 5 PWSC 75.79 165 Note: + tive sign prediction 5. Conclusion:
Prediction method Bergma ASM n
% error ASM
+9.6 69.95 % 71.73 140.1 +0.25 134.20 0 % 73.89 74.3 +1.96 % Under prediction;  tive
Bergma n +7.3% +4.44% +2.50% sign Over
It can be observed in the present study results that the initial crack size, aspect ratio of crack, applied bending stress range, stress ratio, diameter of the pipe are some of the factors affecting the fatigue crack growth life of the piping component. For the material studied in the present case and comparing the results of base and weld metal fatigue crack growth behaviour, it can be concluded that the two fatigue crack growth behaviour compares well.
Fig. 13 Variation of crack length with fatigue cycles
Reference: 14 Prediction ASM Prediction Berg Experimental
Aspect ratio(2c/a)
12 10 8 6 4 2 0 0
10000
20000
30000
40000
50000
60000
Number of cycles
Fig. 14Variation of aspect ratio with fatigue cycles
14
Prediction ASM
Aspect ratio(2c/a)
12
Prediction Berg
10
Experimental 8 6 4 2 0 0
0.2
0.4
0.6
0.8
1
Crack depth/thickness (a/t)
Fig. 15 Variation of aspect ratio with crack depth
Comparison of final crack length
112
[1] ASM Handbook Vol. 19. Fatigue and Fracture. ASM international, the material information society, 1996; Appendices: 9801000. [2] Bergman M. “Stress intensity factors for circumferential surface cracks in pipes” Int. Frac. Engg Mat. Struct., vol. 18, no. 10(1995)1155–1172. [3] Singh PK, Vaze KK, Bhasin V, Kushwaha HS, Ghandhi P, Ramachandra Murthy DS, “Crack initiation and growth behaviour of circumferentially cracked pipes under cyclic and monotonic loading”, Int. Jr. of Pres. Ves. and Piping vol. 80, 2003, pp 629 640. [4] Singh PK, Bhasin V, Vaze KK, Ghosh AK, Kushwaha, RamachandraMurthy DS, Gandhi P and Sivaprasad S. Fatigue studies on carbon steel piping materials and components: Indian PHWRs. Nucl. Engg. Design. 238 (2008) 801813. [5] Andersson P, Bergman M, Bricks B, Dahlberg L, Nilsson F, SattariFar I. A procedure for safety assessment of components with crackshandbook. SAQ/FoU Report 96/08. Stockholm: SAQ Kontrol Lab. 1998. [6] Soni RS, Kushwaha HS, Mahajan SC, Kakodkar A. Qualification of PHT integrated piping system of 500 MWe PHWR Technical report BARC/1998/E/006. [7] E60693, Standard test method for measurement of fatigue crack growth rate. Annual book of ASTM standard, vol. 03.01;1995.
International Journal of Scientific Engineering and Technology www.ijset.com, Volume No.1, Issue No.2 pg:112117
(ISSN : 22771581) 01 April 2012
Table  2.3 Details of the experimental results of surface cracked pip
Notch location
S.No. PWS C126 PWS C 164 PWS C 165
OD mm
t mm
Min.
Stress range (MPa)
Crack Length (2c) mm
Through wall crack cycles
Outer Span mm
Inner span mm
Load (KN) Max
Weld metal
324
21.5
5000
1480
320
32
183
61.2
66000
Weld metal
406
26.5
6500
1600
500
50
196
131
31950
Weld metal
406
26.5
6500
1600
500
50
196
66
50400
Table 4.2 Predicted results using Bergman
a (mm)
2c (mm)
aeff (mm)
2 ceff (mm)
aeff/t
2 ceff / aeff
Ks
5.1
61.2
5.73
61.809
0.2665
10.786
16.18
23.27
17.54
24.754
10.73
63.229
12.32
65.05
0.513
5.31
28.04
37.06
30.554
38.48
58655
17.32
67.2
19.5936
69.012
0.9113
3.522
28.67
44.22
34.75
47.135
11722
21.5
69.9594
Kd
Ks(eff)
Kd(eff)
MPa
Kd
m
MPa
Ks(eff)
m
MPa
Kd(eff)
m
MPa
m
1
dN
2864
a (mm)
2c (mm)
aeff (mm)
2 ceff (mm)
aeff/t
2 ceff / aeff
Ks
5.1
61.2
5.81
61.505
0.27
10.581
12.3
26.63
14.112
28.618
10.8
61.78
11.61
63.226
0.54019
5.4438
26.78
37.75
28.73
39.06
34544
16.6
64.84
18.38
68.385
0.85
3.72
41.69
41.95
44.2
43.23
11099
21.5
71.73
113
1
MPa
m
MPa
m
MPa
m
MPa
m
dN
4782